Solvometallurgy: An Emerging Branch of Extractive Metallurgy
- 3.8k Downloads
This position paper introduces the reader to the concept of solvometallurgy, the term used to describe the extraction of metals from ores, industrial process residues, production scrap, and urban waste using non-aqueous solutions. Here, non-aqueous is not used to imply anhydrous, but rather a low water content. The unit operations are as follows: solvent leaching; separation of the residue; purification of the leach solution by non-aqueous solvent extraction or non-aqueous ion exchange; and metal recovery by precipitation or electrolysis in non-aqueous electrolytes. Solvometallurgy is similar to hydrometallurgy in that both the branches of extractive metallurgy use low-temperature processes, but with solvometallurgy, there is no discrete water phase. Both branches use organic or inorganic solvents (excluding water in the case of solvometallurgy). However, for solvometallurgical processes to be sustainable, they must be based on green solvents, which means that all toxic or environmentally harmful solvents must be avoided. Solvometallurgy is complementary to pyrometallurgy and hydrometallurgy, but this new approach offers several advantages. First, the consumption of water is very limited, and so the generation of wastewater can be avoided. Second, the leaching and solvent extraction can be combined to form a single step, resulting in more simplified process flow sheets. Third, solvent leaching is often more selective than leaching with acidic aqueous solutions, leading to reduced acid consumption and fewer purification steps. Fourth, solvometallurgy is useful for the treatment of ores rich in soluble silica (e.g., eudialyte) because no silica gel is formed. In short, solvometallurgy is in a position to help develop the near-zero-waste metallurgical processes, and with levels of energy consumption that are much lower than those with the high-temperature processes. The Technology Readiness Level (TRL) of this emerging branch of extractive metallurgy is still low (TRL = 3–4), which is a disadvantage for short-term implementation, but offers a great opportunity for further research, development, and innovation.
KeywordsIonometallurgy Lyometallurgy Non-aqueous solvent extraction Solvometallurgy Solvent leaching Sustainable metallurgy
Until a few centuries ago, mankind made use of only seven metals—copper, tin, iron, gold, silver, lead, and mercury—in pure form or in the form of alloys (e.g., bronze) . In the early nineteenth century, metallic zinc began to be produced, although this metal had been used for centuries as a component of brass. All these metals were produced from high-grade ores by the high-temperature, pyrometallurgical processes. However, once the rich ore deposits began to run out, there was no alternative but to start mining lower-grade ores, which could not be processed into a concentrate using the beneficiation methods that were employed at that time. This became a serious problem at the turn of the twentieth century and led to the development of mineral processing (e.g., froth flotation) and hydrometallurgical processing (e.g., leaching, ion exchange, and solvent extraction) . Hydrometallurgy makes use of water as a solvent, and operates at much lower temperatures (20–200 °C) than pyrometallurgy (>300 °C) . Hydrometallurgical processes were originally developed for the extraction of copper and gold, but the extraction of uranium from low-grade ores after World War II gave a boost to the development of hydrometallurgy.
Hydrometallurgical flow sheets are now important for the extractive metallurgy of the rare-earth elements (REEs), zirconium, niobium, tantalum, gallium, indium, platinum-group metals (PGMs) zinc, and copper. The aluminum industry has also contributed to the development of hydrometallurgy; for example, the Bayer process, used to prepare pure alumina from bauxite ore, is the oldest example of a commercialized, high-pressure hydrometallurgical process. For the production of iron, pyrometallurgy is the dominant technique, whereas the flow sheets for the extraction of many other metals are based on a combination of pyrometallurgical and hydrometallurgical process steps. For instance, after sintering and roasting the ore concentrate (i.e., a pyrometallurgical process), the calcine can be leached by an acid (i.e., a hydrometallurgical process). Hydrometallurgy is used only in the first parts of the flow sheet, and metal production is finalized quite often by pyrometallurgy.
In cases where pyrometallurgical or hydrometallurgical processes fail to efficiently extract metal values from low-grade ores, mine tailings, industrial process residues, or urban waste, we could turn to solvometallurgy, which constitutes a branch of extractive metallurgy that is complementary to both pyrometallurgy and hydrometallurgy. Solvometallurgy makes use of processes involving the non-aqueous solvents. These non-aqueous solvents can be molecular organic solvents, ionic liquids, deep-eutectic solvents (DESs), but also the inorganic solvents such as liquefied ammonia, concentrated sulfuric acid, or supercritical carbon dioxide. High-temperature molten salts and liquid metals are excluded if they require temperatures above 300 °C. Non-aqueous solvents do not imply anhydrous conditions, but rather a low water content. Some solvometallurgical processes must take place in the absence of water, while for other processes, a low water content is required. Strictly speaking, conventional solvent extraction, which is based on the preferential distribution of metal ions between an aqueous phase and a water-immiscible organic phase, is not a solvometallurgical process because of the presence of an aqueous phase.
The original concept of solvometallurgy dates from the late 1940s and early 1950s when researchers in the United States were developing processes to recover uranium from the uranium ores through leaching with organic mixtures such as acetone-HCl or alkylphosphoric acids in kerosene [4, 5, 6, 7, 8, 9]. At that time, the term “lyometallurgy” was introduced to describe solvent-based leaching processes, derived from the Greek word lyein, meaning to loosen or to dissolve. Other suggested terms included “anhydrometallurgy” and the contradictory “non-aqueous hydrometallurgy.” Later, solvometallurgical methods were used for the recovery of copper from chrysocolla, a largely amorphous copper silicate [10, 11, 12]. It was also realized that solvometallurgy could be useful for the reprocessing of spent nuclear fuel . Sastri reviewed the possibility of using organic solvents and chelating agents for the processing of ores . In 1985, in his book on ion solvation, Marcus used the term “solvometallurgy” to describe the extension of hydrometallurgy to solvents other than water . Russian researchers also applied the solvometallurgical methods to recover metals from complex silica-rich ores (e.g., eudialyte), urban waste, and pellets of nuclear fuel [16, 17, 18, 19]. In recent years, there has been progress in the use of ionic liquids and deep-eutectic solvents in metallurgical processes, ranging from leaching, to solvent extraction, and the electrodeposition of metals [20, 21, 22, 23]. The term “ionometallurgy” was coined for metallurgical processes involving the ionic solvents , but ionic-liquid processes are solvometallurgical as well. Although we could consider hydrometallurgy to be part of solvometallurgy (since water is a solvent), we want to make a clear distinction between hydrometallurgy (based on water as solvent) and solvometallurgy (based on non-aqueous solvents).
In this paper, we describe the concept of solvometallurgy and its potential applications in extractive metallurgy. An overview of solvometallurgical unit processes is provided, and ten reasons are presented to highlight why solvometallurgy is a useful complement to hydrometallurgy and pyrometallurgy. Because we realize that several hurdles must be overcome before solvometallurgy will become commonplace in extractive metallurgy, the main challenges facing this new approach are discussed. Selected examples of solvometallurgical processes reported in the scientific literature and the patent literature are described. Attention is paid to the selection and disposal of the solvents, because the use of green solvents is a must for the development of sustainable solvometallurgical processes.
Solvometallurgical Unit Processes
Comparison of hydrometallurgical and solvometallurgical processes
Leaching with aqueous solutions of acids or bases, or aqueous solutions of chelating agents
Leaching with acid-saturated neutral or basic extractants, acidic extractants, chelating extractants diluted in nonpolar organic solvents; acid-saturated polar solvents; halogens in organic solvents
Distribution between an aqueous phase and an immiscible organic phase
Distribution between two immiscible organic phases
Ion exchange between the resin and aqueous solutions
Ion exchange between the resin and non-aqueous solutions
Precipitation by reagent addition, control of pH, evaporation of water
Precipitation by reagent addition, addition of anti-solvent, evaporation of solvent
Electrodeposition of metals at the cathode from an aqueous electrolyte
Electrodeposition of metals at the cathode from a non-aqueous electrolyte
In hydrometallurgy, leaching (solid–liquid extraction) mainly involves: (1) mineral acids such as H2SO4, HNO3, or HCl, (2) bases such as NH3 or NaOH, or (3) chelating agents such as EDTA or citric acid. These lixiviants are used in diluted or concentrated forms. In solvometallurgy, one approach to carrying out leaching is with solutions of mineral acids in water-miscible (polar) organic solvents, such as acetone, methanol, ethanol, isopropanol or ethylene glycol [4, 25, 26, 27, 28]. HCl is often selected as the acid. Anhydrous solutions of HCl in an organic solvent can be prepared by saturating the solvent with HCl gas and diluting with solvent until the appropriate HCl concentration. It is also possible to use organic acids such as formic acid or acetic acid in undiluted form or diluted with small amounts of water. Other lixiviants are deep-eutectic solvents (DESs) .
If a neutral extractant such as tri-n-butyl phosphate (TBP) is used, in general the solvent cannot be used directly for the solvent leaching of a solid material, because the neutral extractants are poor lixiviants. However, very powerful lixiviants can be obtained by bringing an organic phase containing TBP into contact with a concentrated aqueous solution of a mineral acid (H2SO4, HNO3, HCl) [13, 30, 31]. During this conditioning step, TBP will extract the acid molecules as well as a certain amount of water. Whereas the extraction of acids by TBP is often an unwanted phenomenon in solvent extraction (because this process competes with the extraction of metal ions), the affinity of TBP for strong acids is an asset during solvent leaching, because a highly acidic organic phase can be obtained. TBP–H2SO4, TBP–HNO3 and TBP–HCl are useful lixiviants in solvometallurgy. TBP can be used in undiluted form or it can be diluted in an organic solvent to reduce its viscosity. The strength of the TBP-based lixiviant can be tuned by varying the acid concentration in the conditioning step. TBP can be replaced by other neutral extractants such as Cyanex® 923, which is a commercial mixture of trialkylphosphine oxides . We could also consider using the 8-hydroxyquinoline derivative Kelex® 100 saturated with mineral acids as a lixiviant . The nitrogen atom in the quinoline ring is relatively basic and has a strong tendency to bind acids. The strong tendency to extract acids is a disadvantage when using Kelex® 100 for conventional solvent extraction, but it is an advantage when using this extractant for solvent leaching.
Basic extractants are anion exchangers, and they are not very suitable for solvent leaching, unless they are combined with mineral acids. In undiluted form, they can be considered as ionic liquids. The ionic liquid trihexyl(tetradecyl)phosphonium chloride (Cyphos® IL 101), saturated with concentrated HCl  as well as the ionic liquid betainium bis(trifluoromethylsulfonyl)imide, [Hbet][Tf2N] have been used to dissolve different metal oxides . Instead of Cyphos® IL 101, a quaternary ammonium chloride such as Aliquat® 336 could also be used.
A promising system for solvent leaching is n-octanol/HCl; this was originally developed by Russian researchers to chemically attack resistant ores such as titanomagnetite . n-Octanol is a cheap solvent and has a very low solubility in water (<0.1%). This system has a low density, resulting in good hydrodynamics and a rapid phase separation from water. The lixiviant is stable over time and is reasonably stable toward concentrated mineral acids. The maximum concentration of HCl in n-octanol is 5.2 mol/L at 20 °C .
In some cases, the dissolution of metal oxides is enhanced by a change in the oxidation state. For instance, MnO2 is much easier to dissolve in an acid solution when a reducing agent is present. An example of a reducing lixiviant for use in solvometallurgy is methanol-HCl [27, 37]. For the dissolution of metals in their elemental state, an oxidative dissolution process is required. This can be achieved with solutions of chlorine, bromine or iodine in organic solvents (vide infra).
Non-Aqueous Solvent Extraction
Solvent extraction (SX) is a very important technique in hydrometallurgy for the separation and purification of metals such as cobalt, nickel, copper, zinc, uranium, REEs, and PGMs . In conventional solvent extraction, the metal ions are distributed between an aqueous phase and a water-immiscible organic phase, in general with the aid of an extractant (also called the extracting agent). Because the various metal ions distribute differently between the aqueous and organic phases, mixtures of metal ions can be separated by solvent extraction. It is clear that an aqueous phase is present in all the hydrometallurgical solvent-extraction processes. This could give the impression that all the solvent-extraction systems must involve an aqueous phase. However, this is not correct: all that is required are two mutually immiscible liquid phases. Solvent-extraction systems can also consist of (1) two mutually immiscible molten salts, (2) a molten salt and a molten metal, (3) a molten salt and an organic solvent, or (4) two mutually immiscible organic solvents.
The solvents at the beginning of the series have a very high polarity, whereas the solvents at the end of the series have a low polarity. Although the miscibility can be tested by simple test-tube experiments, the mutual solubility must be quantitatively measured using Fourier transform infrared (FTIR) spectroscopy, gas chromatography (GC) or nuclear magnetic resonance (NMR) spectroscopy. The mutual solubility is a function of the temperature and the concentration of dissolved salts. Two solvents that are totally miscible in the pure state can phase-separate after the addition of metal salts. For instance, ethanol is miscible with all conventional organic solvents. However, the phase separation of a mixture of ethanol and n-dodecane occurs upon the addition of 1 M LiCl. Higher LiCl concentrations result in the phase separation of mixtures of ethanol and aromatic solvents. Examples of immiscible solvent pairs are methanol–dodecane, formamide–dodecane, acetonitrile–dodecane, and ethylene glycol–dodecane. The ionic liquids 1-ethyl-3-methylimidazolium chloride and trihexyl(tetradecyl)phosphonium bis(2,4,4-trimethylpentyl)phosphinate form a pair of immiscible non-aqueous solvents as well . Another immiscible pair of ionic liquids are betainium bis(trifluoromethylsulfonyl)imide and trihexyl(tetradecyl)phosphonium bis(trifluoromethylsulfonyl)imide . It is important to realize that the extractant dissolved in the less-polar phase can have an influence on the mutual miscibility of the two organic solvents; two solvents that are mutually immiscible can become partly miscible after dissolving an extractant in the less-polar phase. Moreover, some extractants can also extract solvent molecules from the more-polar phase.
Although non-aqueous solvent extraction has not received much attention so far, it offers several advantages over conventional aqueous solvent-extraction systems. First of all, the approach is applicable to the separation of covalent metal compounds such as halide complexes of p-block elements (SiCl4, GeCl4, SbCl3) and early d-block elements (ZrCl4, HfCl4, NbCl5, TaCl5), as well as organometallic compounds. These compounds hydrolyze in water, and the hydrolysis reaction can be vigorous. Second, there is the opportunity to carry out separations that are not efficient in an aqueous solution because of the differences in the extraction mechanism.
Non-Aqueous Ion Exchange
Ion exchange (IX) is an often-used method for the removal of metal ions or metal salts from aqueous solutions. Typically, ion exchanges are carried out using functionalized, crosslinked, polystyrene-derived resins. The strongly acidic cation-exchange resins have sulfonic acid functional groups, whereas the strongly basic cation-exchange resins have quaternary ammonium groups. Whereas solvent extraction is more often used to recover metals from concentrated solutions, ion exchange is typically used for the recovery of metals from dilute aqueous solutions. Many studies have been devoted to the effect of adding polar organic solvents to the aqueous phase, because the presence of an organic solvent can lead to a stronger adsorption of metal ions by the ion-exchange resin and to higher selectivities in separation processes . On the other hand, there are relatively few studies on ion exchange in non-aqueous solvents. Ion-exchange resins must swell in the solvent used in order to adsorb and exchange the ions at a sufficiently rapid rate. In general, ion-exchange resins swell well in water, even if the resin has a relatively high degree of crosslinking. However, commonly used ion-exchange resins might not swell sufficiently in a non-aqueous solvent, leading to a slowing down or inhibition of the ion-exchange reaction. Another reason is that the compounds must exhibit some ionic dissociation, which means that a polar solvent with a relatively high dielectric constant ε r must be used. An exception is anion exchangers with relatively basic anions, which can bind neutral metal complexes through adduct formation. For instance, an anion exchanger in the chloride form can bind nondissociated CoCl2 dissolved in an organic solvent by the formation of a complex anion .
Solvents that can be used instead of water in ion-exchange processes include the lower alcohols (methanol, ethanol, propanol, isobutanol, and n-butanol), polyalcohols (ethylene glycol, propylene glycol, glycerine), ethers (diethyl ether, dioxane, tetrahydrofuran), ketones (acetone, methyl ethyl ketone), organic acids (formic acid, acetic acid), pyridine, DMF and DMSO . To these solvents, mineral acids can be added, for example, H2SO4, HNO3, HCl or HBr. Often, mixtures of these solvents with water are used instead of non-aqueous solvents. However, as mentioned above, the liquid phase must consist of at least 50 vol% of organic solvent if we are to consider the ion-exchange process as a solvometallurgical process. An example of an exotic solvent for ion exchange is molten urea .
A major advantage of non-aqueous ion exchange is that more metal ions form anionic complexes with chloride or nitrate ions in organic solvents than in water, which means that more metals can be recovered using an anion exchanger from an organic solution than from an aqueous solution. A typical example is the trivalent rare-earth ions. These do not form anionic complexes with chloride ions in aqueous solutions and form only anionic complexes with nitrate ions in the presence of very high nitrate concentrations. However, the rare-earth ions readily form anionic complexes with chloride or nitrate ions in organic solvents such as methanol. Other metal ions that only form anionic complexes with chloride ions in organic solvents are thorium(IV), nickel(II), calcium(II) and chromium(III).
Cation exchangers in the protonated (H+) form can be used to recover metal ions from the leachate after direct solid leaching with a solution of a mineral acid in a polar organic solvent, such as HCl in acetone. Anion exchangers in the chloride form can be used to recover metal chloride salts from organic solvents, even from those with a lower polarity, as long as the swelling of the resin is sufficient. Another approach to removing salts from organic solvents is to use dual or mixed beds of cation and anion exchangers .
Precipitation or Crystallization
An alternative approach in hydrometallurgy to the recovery of dissolved metals from the leachate—in addition to solvent extraction, ion exchange or adsorption by activated charcoal—is crystallization or precipitation. Crystallization results from evaporation of the aqueous phase until the aqueous solution becomes saturated and the metal salts start to form crystals. Precipitation can be achieved by increasing the pH to form insoluble hydroxides, or by adding a precipitation agent such as sodium carbonate to precipitate insoluble metal carbonates. Metals can be recovered in metallic form by cementation (for instance by adding iron scrap to a CuSO4 solution) or by reduction with hydrogen gas . In principle, most of these methods can be applied to recover metal salts dissolved in organic solvents, although it is important to realize that water must be present for the precipitation of metal hydroxides. An alternative approach to crystallize or precipitate metal compounds from organic solutions is through the addition of an anti-solvent that is miscible with the solubilizing solvent. It is important to keep in mind that metals must be reduced to the metallic state. Precipitation is needed only if purification or further separation from contaminants is required.
Electrolysis in Non-Aqueous Electrolytes
The electrowinning of metals can be achieved from aqueous electrolytes or from molten salts. It is often used to recover copper, nickel, and zinc from aqueous solutions. A typical example of an electrowinning process based on molten-salt electrolytes is the Hall–Héroult process for producing aluminum metal. Electrolysis can also be used for the electrorefining of metals, by anodic dissolution of the metal and electroreduction of the metal at the cathode. Another use of electroreduction is covering metallic objects with a thin protective or decorative layer of another metal (i.e., electroplating). An example is the coating of a steel plate with a layer of zinc for corrosion protection. Many fundamental studies have been devoted to the electrodeposition of metals from non-aqueous electrolytes, but very few of them have been applied on an industrial scale. There are several reasons for this lack of industrial interest. First of all, non-aqueous electrolytes with dissolved conducting salts have a much lower conductivity with respect to aqueous electrolytes, so that the electrodeposition rates are much slower. Second, there are serious safety issues associated with many organic electrolytes, especially if they are based on volatile solvents such as diethyl ether. Third, sacrificial anodes have to be used, because otherwise the organic solvents in the electrolyte bath will decompose. Most of the technologies developed for the electrodeposition of metals from non-aqueous solvents are about the electrorefining or electrodeposition of metal coatings, not about electrowinning. One of the few examples of the electrowinning of metals from non-aqueous solvents is the electrowinning of zinc and lead from deep-eutectic solvents after the leaching of these metals from electric-arc-furnace (EAF) dust . These deep-eutectic solvents also make it possible to deposit hard chrome layers from chromium(III) salts, which is only possible from carcinogenic chromium(VI) salts when using aqueous electrolytes . The electrodeposition of aluminum layers from non-aqueous electrolytes containing organo-aluminum compounds is applied on an industrial scale by companies such as AlumiPlate Inc. in Minneapolis, MN (www.alumiplate.com) and Rasant–Alcotec in Overath, Germany (www.rasant-alcotec.de). The electrodeposition or electrorefining of metals from non-aqueous electrolytes is interesting for metals that cannot be deposited from aqueous electrolytes, e.g., aluminum, or which can only be deposited with low current efficiencies from aqueous solutions, e.g., germanium. There is a large body of literature on the electrodeposition of metals from ionic liquids, but most of this research is fundamental studies [23, 53, 54].
Organic Solvents for Solvometallurgy
dimethyl formamide (DMF)
cyclopentyl methyl ether
polyethylene glycol (PEG)
dimethyl sulfoxide (DMSO)
polypropylene glycol (PPG)
methyl ethyl ketone (MEK)
methyl isobutyl ketone (MIBK)
diisobutyl ketone (DIBK)
propylene carbonate (PC)
propylene glycol ethers
propylene glycol ethers acetates
(biodegradable) GTL solvents*
Ionic liquids and deep-eutectic solvents are not listed in Table 2 because the properties of these solvents are very much dependent on the composition. The compositional range here is too wide to draw any general conclusions. However, these solvents are often considered as green solvents because of their nonvolatility, low flammability, and, in general, low toxicity.
Volatile solvents might appear to be very useful because they can be recycled by distillation. However, they contribute a great deal to smog formation and present health risks through inhalation. Many volatile solvents have a low flash point, are flammable, and can even form explosive mixtures with air. If possible, distillation should be avoided as a recycling method for organic solvents because this technique is energy intensive and requires the use of volatile solvents. It is, therefore, recommended to explore nonthermal techniques for solvent recuperation rather than distillation. An example of such a technique is organic solvent nanofiltration (OSN), also known as solvent-resistant nanofiltration (SRNF), which is a pressure-driven membrane technique .
The environmental impact of a solvent requires more attention when the solvent is used in a system that is open to the environment, rather than a fully closed system. A solvent used in an open system should be nonvolatile and have a low toxicity. In the case of solvents used for leaching in open systems (e.g., for heap leaching), the biodegradability, i.e., the breakdown of chemical compounds by microorganisms, of the solvent is an asset. Water-soluble esters, ketones, alcohols, and glycol ethers are readily biodegradable, while hydrocarbon solvents often have a much slower biodegradability due to their poor solubility in water, but there are differences in the degradation rate for the different classes of hydrocarbons. The order of susceptibility to biodegradation is: n-alkanes > branched alkanes > low-molecular-weight aromatics > cyclic alkanes. Chlorinated and fluorinated solvents are, in general, poorly degradable. Several ionic liquids have a poor biodegradability, although other types of ionic liquids have been specifically designed to be biodegradable . On the other hand, biodiesel is an easily biodegradable and nontoxic solvent. Biodiesel is a mixture of mono-alkyl esters of long-chain fatty acids derived from vegetable oils or animal fats [62, 63]. It has been successfully tested as a diluent in solvent-extraction studies [64, 65, 66, 67]. Soybean oil methyl esters have also been investigated as a diluent for solvent-extraction systems . Soybean oil consists of a mixture of fatty acids, with the vast majority of the fatty-acid component being linoleic acid, an 18-carbon, long-chain fatty acid with double bonds at carbon atoms 9 and 12. Glycerol is a side product formed during the production of biodiesel, and it is a good solvent for many metal salts . It can also be used as a starting product for the production of other green solvents such as alkyl glycerol ethers .
Methanesulfonic acid (MSA) is an example of a strongly acidic organic solvent that can be considered as a green solvent . Methanesulfonic acid has a low toxicity, is readily biodegradable, and is part of the natural sulfur cycle. In general, metal methanesulfonate salts have a very high solubility in water so that they are often considered as a metal source in the preparation of aqueous electrolytes for metal deposition.
A new class of solvents that shows great promise for applications in solvometallurgy is solvents prepared by gas-to-liquids (GTL) technology . GTL solvents are prepared from natural gas using the Fischer–Tropsch process. The GTL process consists of three stages. In the first stage (syngas reforming), the natural gas is partially oxidized to create synthesis gas (syngas), a mixture of hydrogen and carbon monoxide, which is then purified. In the second stage (the Fischer–Tropsch reaction), the syngas is converted by a catalyst to a long-chain, heavy paraffinic liquid, the Fischer–Tropsch wax, which consists of a mixture of many compounds. In the third stage (product upgrading), the oxygen-containing products and alkenes are hydrogenated to alkanes. Through hydrocracking and isomerization, the paraffins are converted into smaller alkanes with a very characteristic branching pattern. Using distillation, fractions with a different distillation range are obtained. The GTL solvents consist mostly of iso-paraffins and normal paraffins, with only very small amounts of cyclic paraffins. They contain small amounts of impurities such as sulfur, olefins, and polycyclic aromatics. They are almost odorless, due to their low aromatic and naphthenic content. Shell offers a range of commercial GTL solvents with different distillation ranges (GS190, GS215, GS250, GS270, GS310). The solvents with the higher distillation ranges have the lowest volatility, but they also have a higher viscosity (although it must still be considered as a relatively low viscosity). A very interesting property of these solvents is their good biodegradability [73, 74]. GTL solvents were found to exhibit more than 60% biodegradation over the required 28-day test period, with the degradation continuing after the 28 days toward complete degradation. Therefore, they are considered to be readily biodegradable according to the OECD 301F guideline. GTL solvents have better biodegradation scores than comparable petroleum-derived solvents because of the lower proportions of aromatics and/or naphthenics in the GTL solvents.
Organic solvents tend to degrade over time. In general, this is a disadvantage compared with water. In many cases, organic impurities can be removed by a washing step with water or with an organic solvent. In other cases, solvents can be purified by distillation, even though this is an energy-intensive process. This purification process cannot be repeated endlessly, and at any given moment, the solvent has to be replaced by a fresh batch of solvent. At the end of the lifetime of the solvent, safe disposal is required. The best approach is to burn the spent solvent, with heat recuperation. The disposal by incineration is one of the reasons why halogenated solvents must be avoided. Halogenated solvents cannot readily be handled in most incinerators.
Although inorganic solvents (with the exclusion of water, of course) can in principle be used for solvometallurgical processes, inorganic solvents are generally of little use in this context because they are too reactive, too dangerous, too toxic or too difficult to handle. Examples include liquid ammonia, liquid sulfur dioxide, anhydrous hydrogen fluoride, thionyl chloride, sulfuryl chloride, phosphoryl chloride, dinitrogen tetroxide, and antimony trichloride. Concentrated sulfuric acid is an inorganic solvent, but it is not used in solvometallurgy as a solvent, but rather for ore acidification (acid curing of ores). Supercritical CO2 could find applications in the field of non-aqueous solvent extraction and solvent leaching [75, 76, 77, 78]. Of particular interest are the promising combinations of supercritical CO2 with TBP-HNO3 and supercritical CO2 with fluorinated β-diketones as solvents for direct solid leaching [79, 80, 81, 82, 83]. CO2 becomes a supercritical fluid at its critical temperature (31.10 °C) and critical pressure (72.8 atm) . Any supercritical fluid expands to fill a container, but it has a density that is similar to that of a liquid.
Ionic Liquids (ILs) and Deep-Eutectic Solvents (DESs)
Although the physicochemical properties of ionic liquids are very dependent on the chemical composition of the ionic liquid, we can also make some generalizations. First of all, many ionic liquids have a nonmeasurable vapor pressure at room temperature, although some ionic liquids can be distilled in a high vacuum at high temperatures. Ionic liquids often have a very wide liquidus range; it is not uncommon to have ionic liquids that are fluid over a range of more than 250 °C, which is much wider than the 100 °C range of water. Ionic liquids are intrinsic electrical conductors, and they can have an electrochemical window of more than 4 V (the electrochemical window of water is just 1.23 V). Ionic liquids are good solvents for many classes of inorganic and organic compounds. Compared with molecular organic solvents, ionic liquids have a much higher viscosity, which can hamper mass transport and slow down the rate of chemical processes. However, the viscosity of ionic liquids reduces dramatically upon heating or the addition of a small amount of a molecular co-solvent.
A drawback of many ionic liquids is their high price, and this has hindered the development of ionic-liquid processes on an industrial scale. A cheap alternative to ionic liquids are the deep-eutectic solvents (DESs) [22, 29, 89, 90], of which there are many different types. Most of them are mixtures of choline chloride and a hydrogen-bond donor (urea, ethylene glycol, malonic acid) or mixtures of choline chloride with a hydrated metal salt. A typical feature of a DES is that it has a much lower melting point than each of its individual components. Popular DESs are those obtained by mixing chloride and urea in a 1:2 molar ratio, or choline chloride and ethylene glycol in a 1:2 molar ratio. These solvents are liquid at room temperature. Choline chloride is produced on a large scale and is used as chicken feed. Due to the low cost of DESs, it is much easier to use them on a large scale than ionic liquids. Although DESs often have a significant water content, their properties are generally different from those of aqueous solutions. As mentioned before, hard chrome layers can only be electrodeposited from aqueous electrolytes using toxic chromium(VI) salts, whereas the metal can be deposited from DESs containing the much-less-toxic chromium(III) salt. In fact, a DES electrolyte for chromium deposition can be prepared by simply mixing CrCl3·6H2O and choline chloride , or by mixing CrCl3·6H2O and urea . Although deep-eutectic solvents cannot be considered as ionic liquids, as they are mixtures of ions and smaller or larger amounts of neutral molecules, their properties are very similar to those of conventional ionic liquids. For this reason, they are often described as ionic-liquid-like solvents, or just as ionic liquids. Due to their water content, the electrochemical window of DESs is smaller than that of conventional ionic liquids.
The most obvious applications for ionic liquids and deep-eutectic solvents in solvometallurgy are in the electrodeposition of metals from non-aqueous electrolytes. Commonly used ionic liquids for electrodeposition are 1-butyl-3-methylimidazolium bis(trifluoromethylsulfonyl)imide, [C4mim][Tf2N], or N-butyl-N-methylpyrrolidinium bis(trifluoromethylsulfonyl)imide, [BMP][Tf2N], as well as several deep-eutectic solvents . Other applications of these ionic solvents in solvometallurgy are as solvents for solvent leaching and in non-aqueous solvent extraction. As mentioned in the introduction, the term “ionometallurgy” is used for solvometallurgical processes based on ionic liquids or deep-eutectic solvents .
Ten Good Reasons to Use Solvometallurgy
Ten good reasons to use solvometallurgy
Reason 1. Very limited water consumption
Reason 2. Reduced energy consumption
Reason 3. Process intensification
Reason 4. Reduced consumption of acids
Reason 5. Higher selectivity for leaching
Reason 6. Fewer problems with silica gel formation
Reason 7. Suitable for the treatment of low-grade ores, mine tailings, and industrial process residues
Reason 8. Useful for the treatment of urban waste
Reason 9. Compatibility with bioleaching
Reason 10. New separation processes
Reason 1. Very Limited Water Consumption
Because no bulk aqueous phase is present in a solvometallurgical process, the consumption of water can be limited to a strict minimum. In some solvometallurgical processes, a small amount of water is essential, but the water volumes are always small compared to the volumes of organic solvents, and in most cases no discrete aqueous phase is present. If no water is consumed in a solvometallurgical process, it also implies that no wastewater is generated, and that there are no issues with wastewater treatment. Solvometallurgical processes have the potential to recover metals from ore deposits in arid areas, where it is difficult to guarantee a sufficient supply of process water. This is very relevant for exploiting copper mines in the Atacama Desert in Chile. Likewise, solvometallurgical processes can also be operated in (mobile) stand-alone units that can be used to recover metals from small ore deposits at remote locations.
Reason 2. Reduced Energy Consumption
Solvometallurgical processes offer the opportunity to treat, at ambient temperatures, ores that otherwise have to be heated to high temperatures to convert them to oxides before they can be further processed. A good example is the calcination of carbonate ores. By means of chlorine gas dissolved in an organic solvent, it is possible to chlorinate ores at ambient temperatures, instead of using chlorination or carbochlorination at high temperatures. The possibility to work at room temperature or at slightly elevated temperatures results in a considerably reduced energy consumption compared with pyrometallurgical processes, which are typically carried out at temperatures above 300 °C. In general, organic solvents have a lower heat of vaporization than water, so that less energy is required to distil the organic solvent (for solvent recycling) than to distil the same volume of water. However, as mentioned elsewhere in this paper, the use of volatile organic solvents and distillation must be avoided, whenever possible.
Reason 3. Process Intensification
Solvometallurgy allows for process intensification, because different unit operations (e.g., leaching and solvent extraction) can be combined, and this reduces the number of process steps. A combination of mechanical activation (e.g., by ball milling) and solvometallurgy allows the treatment of resistant ores such as columbite, tantalite, and pyrochlore under much milder conditions (ambient temperatures, no HF) with respect to traditional metallurgical methods .
Reason 4. Reduced Consumption of Acids
Even if acid curing of the ore is used as a pretreatment step prior to solvent leaching, the total acid consumption can be much lower than that in the case of conventional leaching. This is because a larger excess of acid is often used in conventional acid leaching and because protons can be provided by the extractant in the case of solvent leaching with acidic extractants. Hydrometallurgical processes with acid leaching are not very compatible with carbonate-rich ores and especially not with those rich in calcite or dolomite, because the dissolution of the carbonate gangue material consumes large amounts of acids. This is relevant if the minerals in a carbonate matrix cannot be separated from the gangue by flotation, e.g., in the case of the uranium ore carnotite. By solvent leaching the ore minerals, the carbonate gangue materials can be left largely untouched. Because solvent leaching is more selective than leaching with aqueous solutions of mineral acids, it is possible to avoid the co-dissolution of unwanted metals such as iron, which also leads to a reduction in the consumption of acids (see also Reason 5).
Reason 5. Higher Selectivity for Leaching
In general, leaching with aqueous solutions of mineral acids (H2SO4, HNO3, HCl) suffers from low selectivity. Besides the targeted metals, many unwanted metals are co-dissolved. This poor selectivity leads not only to a higher consumption of acids (see Reason 4), but also to extra process steps for the removal of impurities from the leachate. Solvent leaching can, in principle, offer a higher selectivity than leaching with aqueous solutions of acids, especially if chelating extractants are used, such as the LIX® family of extractants.
Reason 6. Fewer Problems with Silica Gel Formation
For the recovery of technological metals such as rare earths, zirconium, tantalum, or niobium, we are forced to rely more and more on ores with a complex composition and a high content of soluble silica, because of the depletion of ores with a simpler chemical composition. A good example is eudialyte, Na15Ca6(Fe,Mn)3Zr3(Si,Nb,REE)Si25O73(OH,Cl,H2O)5. The leaching of such minerals with mineral acids dissolves the silica as silicic acid. This dissolved silica is gradually transformed by polymerization into colloidal silica, and these colloids can aggregate to form a gel. Gel formation in a leachate makes the filtration for solid–liquid separation impossible. Dissolved silica can also interfere with solvent extraction, because it causes the formation of extremely stable emulsions during the mixing of the aqueous and the organic phases. These emulsions can be stable for weeks or even months. Silica colloids can also block the pores in ion-exchange resins. Dissolved silica is not only a problem in the case of acidic leaching; it is even more so in the case of alkaline leaching, because silica has a higher solubility in alkaline solutions. Because water is required for the formation of silicic acid, it is evident that the leaching of silica-rich ores with non-aqueous solvents leads to much lower solubilization of the silica and hence to fewer problems with silica gel formation.
Reason 7. Suitable for the Treatment of Low-Grade Ores, Mine Tailings, and Industrial Process Residues
As mentioned in the introduction, the depletion of high-grade ores with a simple composition necessitates the shift to low-grade ores, mine tailings, and industrial process residues that contain only low concentrations of valuable metals and often have a complex composition with several mineral phases. Conventional leaching with aqueous solutions of mineral acids lacks selectivity, leading to the consumption of large amounts of acid and the co-dissolution of unwanted impurities. In particular, the co-dissolution of the matrix is a major problem. Solvometallurgical processes are suitable for the recovery of metals from low-grade ores (e.g., nickel laterites), tailings from primary mining, or industrial process residues (e.g., bauxite residue, goethite, or jarosite) because of their intrinsic higher selectivity (see also Reasons 4 and 5).
Reason 8. Useful for the Treatment of Urban Waste
In ore deposits, the metals typically occur in complex polymetallic sulfide or oxide ores, whereas the metals of the urban mine are typically present in the form of alloys. Examples are the rare-earth permanent magnets, which consist of neodymium-iron-boron or samarium-cobalt alloys. The direct reuse of these alloys is often not possible, and the mixture of constituting metals needs to be separated into the individual elements. In hydrometallurgical recycling methods, the alloys are dissolved in aqueous solutions of strong mineral acids (H2SO4, HCl, HNO3). This step can be unsafe because of the formation of flammable hydrogen gas during the metal dissolution. In the case of arsenic-containing alloys (e.g., GaAs), there is a danger of formation of highly toxic arsine gas (AsH3). The acidic attack dissolves the whole mass of the alloy, so that selective leaching is impossible, and large volumes of acid are consumed. This is a problem with the recovery of rare earths from neodymium-iron-boron magnets, since 70 wt% of the magnet alloy consists of iron. The pyrometallurgical recycling of metals often involves a high-temperature chlorination step to transform the metals into the corresponding chlorides, followed by fractional distillation or sublimation, or by further hydrometallurgical processing (e.g., solvent extraction) after the dissolution of the chlorides in water. This approach is not energy efficient, and it is difficult to obtain high-purity compounds by distillation or sublimation. The hydrometallurgical process steps make the flow sheet more complicated, and they can be carried out only in very acidic solutions to avoid hydrolysis and the precipitation of the metals. After purification by solvent extraction, the dissolved metals have to be converted into anhydrous chlorides, fluorides, or oxides before they can be further processed to the metal, for instance, by electrolysis in molten salts. The flow sheets for the recycling of valuable metals from production scrap and end-of-life consumer goods (Fig. 1) can be shortened and made to be more energy efficient by using solvometallurgy if (1) the chlorination is carried out with chlorine gas dissolved in an organic solvent rather than in a chlorine gas stream at high temperatures, (2) the water in the hydrometallurgical process steps is replaced by organic solvents, and (3) the electrolysis is carried out in organic electrolytes instead of molten salts.
Reason 9. Compatibility with Bioleaching
Although the aim is to recover 100% of the organic solvent after the solvent leaching, complete recovery of the solvent is impossible and some traces of solvent will always remain adhered to the particles of the solid residue, even after a washing step with another organic solvent. However, the solid residue obtained after the solvent leaching can be treated in a subsequent step with bioleaching. This bioleaching step can further enhance the recovery of metals from the residue. Based on differences in the reactivity between the solvent leaching and the bioleaching steps, metals other than those solubilized in the solvent-leaching step can be solubilized in the bioleaching step. More importantly, the solvent traces left after solvent leaching are rich in carbon and could serve as a nutrient for heterotrophic microorganisms (bacteria and fungi), which need organic supplements for growth and energy supply. In this way, the solid residue can be cleared from any solvent traces left behind after the solvent leaching. It is of course necessary that the solvents used for the solvent leaching are not toxic to microorganisms. Of course, it is preferable for the solvents to be biodegradable. Nonpolar solvents with a good biodegradability include some gas-to-liquid solvents (GTL solvents) prepared using the Fischer–Tropsch synthesis from natural gas, such as the GS series of solvents produced by Shell (e.g., GS250). In addition, biodiesel could be used as a biodegradable nonpolar solvent in solvometallurgical processes.
Reason 10. New Separation Processes
Some separation processes can only be carried out in the absence of water. An example is the electrowinning of reactive metals in non-aqueous electrolytes (electrodeposition of aluminum or very pure indium), which is possible in high-temperature molten salts, but not in aqueous solutions. Another example is the purification of LiCl [19, 93], which is very soluble in many organic solvents, in contrast to the other alkali-metal chlorides. Alcohols are particularly good solvents for LiCl, due to the formation of stable solvates such as LiCl·3CH3OH in methanol or LiCl·4C2H5OH in ethanol. By treating mixtures of alkali-metal chlorides with absolute ethanol, LiCl goes into solution, whereas NaCl and KCl do not.
Examples of Solvometallurgical Processes
Solvent Leaching of Low-Grade Uranium Ores
The acetone-HCl process is based on the high solubility of uranyl chloride in acetone [4, 94, 95]. The ore is crushed to 10 mesh and first treated with concentrated HCl or with a mixture of concentrated HCl and H2SO4 to solubilize uranium. The cured ore is fed into a pool of acetone in an enclosed extractor. Uranium, iron, vanadium, and calcium are dissolved in acetone as chloride complexes. Anhydrous ammonia gas is bubbled through the loaded acetone phase, and the dissolved metals precipitate as hydroxides. The hydroxide precipitate is removed by filtration, and the regenerated acetone is returned to the extractor. The final concentrate is of a low grade and contains about 10–15% U3O8. Since acetone is not selective for uranyl chloride dissolution, the process is used primarily for upgrading low-grade ores. The advantage of the process is the small volume of water required. Therefore, the process could be useful for upgrading ores using relatively small installations in remote areas. The disadvantages are that a gas-tight system is needed to minimize the acetone losses and that HCl is required. HCl is more expensive than H2SO4 and it causes more corrosion problems. The precipitated hydroxides are bulky and of low grade.
The alkyl phosphoric acid process uses alkyl phosphoric acids and H2SO4 for the extraction of uranyl ions from the ores [5, 9]. This process is well suited to the recovery of uranium from high-lime carnotite ores. The process was optimized for OPA, a mixture of mono- and dialkylphosphoric acids, but other alkyl phosphoric acids such as bis(2-ethylhexyl)phosphoric acid (D2EHPA) can be used as well. The ground ore is passed on a moving belt, and a solvent is sprayed on it. The solvent is an acidified solution of an alkyl phosphoric acid in a diluent. The solvent percolates through the ore bed and dissolves the uranium. The solvent entrained by the solid residue is washed with fresh diluent at the discharge end of the moving belt. This solvent-leaching strategy is highly dependent on several process parameters. The most important parameters are the type and concentration of the solvent, the amount and type of the acid, the type of diluent, the phase ratio of solvent to ore, and the contact time during the leaching. The contact time can be short, i.e. 10–20 min. The preferred acid is H2SO4, and concentrated H2SO4 (96%) is used to reduce the amount of water. Upon reacting the H2SO4 with the ore, a coating of CaSO4·2H2O (gypsum) is formed around the calcite particles. This isolates the calcite particles and prevents any further consumption of H2SO4. On the other hand, the coating of uranyl sulfate formed on the surface of the uranium minerals can be dissolved by the organic solvent. The freshly exposed surface of the uranium mineral particles further reacts with H2SO4 and the process continues until the entire uranium mineral particle is dissolved. Only about one-tenth of the stoichiometric amount of H2SO4 that would be required to dissolve all of the uranium minerals and calcite is needed. For this reason, the alkyl phosphoric acid process is very suitable for the recovery of uranium from high-lime carnotite ore. The amount of H2SO4 that is used also affects the loss of alkyl phosphoric acid to the solid residue. When no H2SO4 is used, a considerable amount of alkyl phosphoric acid is deposited on the ore, and this cannot be recovered by washing the residue with a diluent. The best efficiencies are observed by adding H2SO4 to the solvent before or during the contact of the solvent with the ore. Acid curing of the ore before contact with the solvent causes local neutralizations and the consumption of larger amounts of acid. The best uranium recoveries are obtained with methyl ethyl ketone (MEK) as the diluent, but isopropyl ether (IPE) has a lower solubility in water. Although kerosene would be a desirable solvent because of its low solubility in water and its relatively high flash point, the use of kerosene results in slow slurry-settling rates, higher alkyl phosphoric acid losses, and more difficult solvent recovery from the solid residue. In the final step, uranium can be stripped from the loaded solvent using a 10 M HCl solution.
Solvent Leaching of Copper Ores
One of the principal oxidized copper ores is chrysocolla, which is a poorly defined hydrated copper(II) silicate with varying composition, often represented by the formula CuSiO3·2H2O. The recovery of copper from chrysocolla by direct acid leaching is challenging because of the formation of silica gel. Raghavan and Fuerstenau developed a solvometallurgical process for the recovery of copper from chrysocolla by leaching it with the extractant LIX® 63 dissolved in kerosene, in the presence of a small amount of aqueous ammonia solution [10, 11, 12]. LIX® 63 is a selective extractant for the extraction of copper from ammoniacal solutions and its active component is 5,8-diethyl-7-hydroxy-6-dodecanone oxime. The authors were able to leach 70–75% of the copper from the ore using an ammonia content that is only about one-quarter of the stoichiometrically required amount for leaching with ammoniacal solutions. The facts that chrysocolla is a porous solid and that the pores are filled with capillary condensed water are crucial to the success of the method. Removal of the water from the pores by heating led to much lower leaching efficiencies. The nonporous synthetic CuO gave poor results as well. Ammonia is believed to enter the pores and react with the copper(II) to form the [Cu(NH3)4]2+ complex, which diffuses to the entrance of the pores on the surface of the ore particles where it reacts with LIX® 63 dissolved in kerosene. Ammonia is regenerated during this reaction and returns to the aqueous phase within the pores. This process was also applied to ocean-floor manganese nodules to recover copper, nickel and cobalt, but the leaching efficiencies were poor unless a reductive treatment at 600 °C was first applied. In that case, a recovery of 71% for nickel, 69% for copper, and 44% for cobalt could be achieved.
The solubility product of Cu2S in acetonitrile is a factor of about 1040 higher than the corresponding value in water (about 10−25 in a 1-M H2SO4 at 25 °C). The driving forces are the strong solvation of the Cu+ ion in acetonitrile and the poor solvation of the H+ ion in acetonitrile. After the dissolution the copper can be recovered from the solution by the addition of water so that Cu+ disproportionates into Cu2+ and Cu. The H2S can be oxidized to H2SO4, which can then be used in the leaching process. Not only Cu2S, but also NiS and AgS are soluble in acidified acetonitrile, but these processes have not yet been investigated in detail.
Acetonitrile is recovered by distillation, and this leads to the disproportionation of copper(I). The advantage of this method is that the SO2 can be converted into sulfate, which means that the method can be coupled with the roasting of sulfidic ores. In general, a roasting plant has to be coupled to a sulfuric acid plant to avoid the release of SO2 to the atmosphere. In this case, the SO2 can be used for the reductive dissolution of metal oxides, such as CuO. Parker and coworkers have investigated the metallurgical applications of copper(I) in acetonitrile–water solutions in detail (cuprous metallurgy) [98, 99, 100].
A remark has to be made about acetonitrile and other organic nitriles. Although these compounds contain the cyano group (−CN), they do not behave like ionic cyanides such as NaCN or KCN, which release the highly toxic hydrogen cyanide (HCN) gas when in contact with acid. Organic nitriles are relatively stable compounds, but they can be metabolized to hydrogen cyanide. However, the metabolism of acetonitrile is much slower than that of other aliphatic nitriles (propionitrile, butyronitrile, acrylonitrile) so that acetonitrile has a relatively low toxicity [101, 102].
The dissolution of chalcopyrite (CuFeS2) in acidic aqueous solutions at near-ambient temperatures and at atmospheric pressure proves to be a challenge because of the surface passivation. For this reason, the leaching of chalcopyrite is typically performed under oxidizing conditions or at high temperatures and pressures. Solis-Marcial and Lapidus found that the formation of a passivation layer could be limited by leaching with H2SO4/H2O2 in the presence of acetone or ethylene glycol in the aqueous phase . The enhanced recovery of copper was attributed to the greater stability of the copper(I) ion in organic solvents. In a follow-up study, those authors investigated the leaching of chalcopyrite by H2SO4 in the presence of alcohols (methanol, isopropanol) using different oxidants (H2O2, CuSO4, O3) . Also, the addition of acetic acid instead of an alcohol resulted in good copper extraction, but the addition of formic acid did not . This negative result can be explained by the oxidative degradation of formic acid by the oxidizing agents.
Recovery of Zinc From Industrial Process Residues
A solvometallurgical process has been developed for the recovery of zinc from different chloride-containing solid residues: zinc ash from galvanizing baths, and flue dusts from the zinc smelting and Waelz processes . The zinc ash is formed when the molten metallic zinc in a galvanizing bath is oxidized on the surface of the bath. This zinc ash, which floats on top of the molten zinc, is a mixture of zinc oxide and small metallic zinc particles. It contains various impurities (e.g., iron and lead), but also relatively large amounts of chloride compounds originating from the chloride fluxes used in the galvanizing process. The zinc flue dusts are formed in different pyrometallurgical processes such as the zinc smelting and Waelz processes, in which the zinc is volatilized after the reduction of zinc-containing materials by carbon in a rotary kiln. The flue dusts consist mainly of ZnO, but also contain oxides of lead, tin, copper, and iron, as well as zinc chloride. The solvometallurgical process is based on the reaction of the fine-grained zinc oxide with acidic extractants, and in particular with carboxylic acids such as naphthenic acids and Versatic acid. The carboxylic acids are used as a 30% solution in an aliphatic diluent. The co-dissolved chlorides can be easily scrubbed from the organic phase by washing with water. After this washing step, the organic phase is chloride-free and contains only the dissolved zinc carboxylate salt. Zinc can be stripped from the loaded organic phase by H2SO4, resulting in an aqueous solution of ZnSO4, from which zinc metal can be recovered by electrolysis. Alternatively, the ZnSO4 can be obtained in crystalline form (ZnSO4·7H2O) by stripping the organic phase with an excess of H2SO4. After the stripping of zinc from the organic phase by H2SO4, the carboxylic acid is regenerated and returned to the process for leaching a new batch of zinc-containing solid material. After the leaching, the solid residue is freed from contaminating organic material by a wash with hot water and with a Na2CO3 solution. The residue after the leaching of the zinc ash contained mainly metallic zinc particles. The solid residue obtained after leaching of the flue dust was very rich in lead.
The leaching step with Versatic acid can be combined with a solvent-extraction step to separate the zinc from the iron [107, 108]. Zinc calcine obtained by roasting zinc oxide was leached with a 30% solution of Versatic acid in an aliphatic diluent. After a subsequent contact between the zinc-containing organic phase and an iron-containing aqueous zinc sulfate solution, an exchange between the zinc and iron takes place. The iron is thereby transferred to the organic phase, where it is present as an iron(III) versatate complex. With this exchange, an equivalent amount of zinc passes from the organic phase into the aqueous zinc sulfate solution. In this manner, the iron is removed completely from the zinc sulfate solution through a contact between the two immiscible phases in one or more stages depending on the technical procedure of the liquid–liquid extraction process. Iron can be stripped from the organic phase by bringing it into contact with sulfuric acid or another mineral acid in one or more stages. Versatic acid can thereby be regenerated into its acid form and is again ready to be loaded with zinc when reacted with solid ZnO (calcine). Instead of Versatic acid, other acidic extractants such as D2EHPA can be used. This approach is not limited to the removal of iron from zinc sulfate solutions; it is also possible to separate zinc from copper.
Recovery of Metals From Complex Ores
During the past two decades Russian researchers have developed several processes for the recovery of valuable metals from refractory ores and ores rich in soluble silica (e.g., eudialyte) that are difficult to treat using conventional hydrometallurgical processes [17, 19]. A common feature of these solvometallurgical processes is the combination of mechanical activation with solvent leaching. It was found that the leaching efficiency was considerably improved with this mechanical activation step. The mechanical activation can be performed before the leaching step, but the two steps can also be combined into a single step, by grinding the ore in the presence of the reactive solvent. Reactive grinding can be considered as a type of mechanochemical reaction. Mechanical activation can be carried out by ball milling. The mechanical preactivation of the ore before bringing it into contact with the solvent seems to be the most promising one.
The combination of mechanical activation and solvent leaching with TBP–HNO3 was used to extract the rare earths and zirconium from eudialyte . Eudialyte becomes more amorphous during mechanical activation and this strongly affects the tendency of metal ions to be leached from the ore. It was found that mechanical activation for a short period of time (0.5–3 min) was particularly effective in improving the recovery of the metals. The mechanical activation was associated with static distortions of the crystal lattice and the rearrangement of large structure-forming cations. Interestingly, prolonged activation led to poorer leaching efficiencies compared with the leaching of the nonactivated ore. In the absence of water, the silica from the eudialyte does not form silicic acid or nonfilterable silica gel, but the silica was released in larger aggregates, which could be easily filtered.
A solvometallurgical process was developed for the recovery of uranium and vanadium from refractory brannerite ore . In the first step, the granulated ore was treated with concentrated H2SO4 at 250 °C. In the second step, the sulfated product was leached with a mixture of 0.1-M bis(2-ethylhexyl)phosphoric acid (D2EHPA) and 0.1-M tri-n-butylphosphate (TBP) in tetrachloroethylene (TCE). It was found that leaching could be achieved only by the addition of a small amount of water, which is needed to form an invisible layer on the surface of the solid particles (wetting of the surface). Of course, the use of the halogenated solvent TCE is not recommended.
Kopkova has found that a titanomagnetite concentrate could be decomposed by an organic solvent consisting of n-octanol saturated with concentrated HCl . Titanomagnetite has an inverse spinel structure and is very resistant to chemical attack, but it could be a potential resource for titanium and vanadium. Besides titanomagnetite, the concentrate also contained antigorite, amphibole, and ferroactinolite. By treating the ore concentrate with n-octanol/HCl, FeCl3 and vanadium chlorides were extracted to the organic phase, while titanium oxychloride remained in the aqueous microphase that was formed in situ. This aqueous microphase is a crucial part of the solvometallurgical process. Water is formed in the chemical reaction between the metal oxide and HCl. This water is separated from the n-octanol phase.
Ionometallurgy makes use of ionic liquids as solvents. A cyanide-free leaching system based on ionic liquids was developed for the recovery of gold and silver from sulfidic ores consisting of chalcopyrite, pyrite, and pyrrhotite [110, 111]. The room-temperature ionic liquid 1-butyl-3-methylimidazolium hydrogensulfate, [BMIM][HSO4] was used as the solvent for the leaching agent thiourea and the oxidant Fe2(SO4)3. The recovery of gold at 50 °C was similar to that of the aqueous system H2SO4/thiourea/Fe2(SO4)3 (≥85%), but the recovery of silver was significantly higher (≥60%). The ionic liquid could be recycled after the selective stripping of gold and silver by activated charcoal. Reuse of the ionic liquid in four successive ore-treatment steps did not lead to degradation of the ionic liquid or lower recovery yields. Ionic liquids with a longer alkyl chain than the butyl chain in [BMIM][HSO4] gave poorer recovery yields, and this was attributed to the higher viscosity of these ionic liquids, resulting in a slower mass transfer. [BMIM][HSO4] also allowed for an efficient recovery of copper (~85%) from chalcopyrite, with the limited co-dissolution of iron (~8%) . The most efficient lixiviant for copper recovery was 100% [BMIM][HSO4]; the addition of water decreased the recovery yield. The selective recovery of gold and silver could also be achieved with the ionic liquid 1-butyl-3-methylimidazolium chloride, [BMIM]Cl, in combination with sodium iodide (NaI) and potassium peroxomonosulfate (KHSO5, Oxone®) . The ionic liquid [BMIM][HSO4] was found to be effective for the leaching of copper from chalcopyrite at temperatures from 70 to 90 °C, but not below 70 °C . This suggests a high activation energy for the leaching reaction. Dissolved oxygen is required for the oxidative dissolution of chalcopyrite. With optimized parameters, 88% of the copper could be recovered. The oxidative leaching of chalcopyrite was carried out with [BMIM][BF4] using Fe(BF4)3 as the oxidant . Leaching was faster in the ionic liquids than in water, even if the ionic liquid was diluted with water. The rapid recovery of copper (45% Cu dissolution after 30 min) was observed in vacuum conditions at 100–120 °C, where water and sulfur were removed to a cold trap. Electrum (AuAg alloy), galena (PbS), chalcopyrite (CuFeS2), and tellurobismuthite (Bi2Te3) could be dissolved in the deep-eutectic solvent choline chloride:ethylene glycol (1:2) (Ethaline®), using iodine as the oxidizing agent . Pyrite (FeS2), calaverite (AuTe2), sperrylite (PtAs2), and moncheite (PtTe2) could not be dissolved under these conditions, but preliminary tests showed that they could be dissolved in this deep-eutectic solvent by electrolysis (anodic dissolution).
Bauxite residue (also known as red mud) is the solid-waste residue formed during the extraction of alumina from bauxite using the Bayer process. The main components of bauxite residue are Fe2O3, SiO2, Al2O3, and TiO2, but bauxite residue also contains significant concentrations of rare-earth elements (REEs) and especially scandium. In fact, bauxite residue could become a major source of scandium . The ionic liquids 1-ethyl-3-methylimidazolium hydrogensulfate, [EMIM][HSO4] and betainium bis(trifluoromethylsulfonyl)imide, [Hbet][Tf2N] were used for the high-temperature leaching of bauxite residue [117, 118, 119]. The leaching parameters were optimized to maximize the REE recovery, while reducing the co-dissolution of iron. [Hbet][Tf2N] was found to be the most suitable ionic liquid, because the REE can be easily stripped from this water-immiscible ionic liquid by an acidic aqueous solution and at the same time, the ionic liquid is regenerated. A disadvantage of this process is the high price of the fluorinated ionic liquid [Hbet][Tf2N].
The ionic liquid [BMIM]Cl and the deep-eutectic solvent choline chloride:urea (1:2 molar ratio) were used for the recovery of REEs from coal byproducts using ion exchange, but the ionic liquid and the deep-eutectic solvent did not show any advantages over leaching with an aqueous ammonium sulfate solution .
[BMIM][HSO4] was tested for the recovery of copper and zinc from brass ash (brass dross) . The brass ashes consisted mostly of metal oxides (ZnO, CuO), although a significant part of the copper was present as metallic particles. Zinc almost completely dissolved in a 50 wt% [BMIM][HSO4] solution in water without any added oxidant, but the recovery of copper was low. The addition of H2O2 to the ionic-liquid solution led to an 82% recovery of copper, and at the same time the dissolution of zinc was found to be faster. After the dissolution of ZnO in the ionic liquid [BMIM][HSO4] without added oxidant, metallic zinc could be recovered from the leachate by electrodeposition . Tests with the protic ionic liquid 1-methylimidazolium hydrogensulfate showed that aqueous solutions of the ionic liquid gave a better recovery of zinc and copper than the concentrated ionic liquid . [BMIM][HSO4] was used for leaching copper from waste printed-circuit boards (WPCBs) . An almost complete recovery of copper was possible with 30% H2O2 as the oxidizing agent.
Deep-eutectic solvents (DESs) have been explored for the selective dissolution of metals from mixed-metal oxides . Different types of DESs showed different types of behavior for dissolving metal oxides. The solubilities of a series of 3d transition-metal oxides in DESs based on malonic acid, urea, and ethylene glycol have been compared . In general, the malonic-acid-based DESs showed the highest solubility for metal oxides. The DES choline chloride:oxalic acid (1:1) can solubilize up to 0.341 mol/L of Fe3O4 at 50 °C. A process has been developed to extract the lead and zinc from electric arc furnace (EAF) flue dust, originating from the remelting of steel scrap [51, 127]. The dust forms when volatile metals such as lead and zinc are vaporized at the high operating temperature of the EAF. About 15–20 kg of dustis formed per ton of steel. The DES choline chloride:urea (1:2) can selectively dissolve zinc oxide and lead oxide, while having a negligible solubility for iron oxides . After the dissolution, lead and zinc could be recovered by electrodeposition. However, the high viscosity of the DES (~800 cP at 25 °C) resulted in impeding the pumping and a more difficulty in the separation of the DES from the undissolved solids by filtration. The viscosity could be reduced by adding ethylene glycol to the DES . A DES with the composition choline chloride: ethylene glycol: urea in the molar ratios 1:1.5:0.5 had a viscosity of 56 cP at room temperature. A dust loading of up to 7 wt% was used, with a digestion time of at least 24 h. Hardly any iron was co-dissolved (<1 ppm). Lead was recovered from the DES by cementation with zinc dust, and ZnCl2 could be precipitated by adding an NH3 solution. The electrowinning of zinc showed that the process was very slow and that the current efficiency was low. The I2/I− redox couple is a strong oxidizing agent in the DES choline chloride: ethylene glycol (1:2 molar ratio) . A process has been developed to dissolve polymetallic waste using an electrocatalytic oxidation by iodine . After the oxidation, the iodide is reoxidized to iodine at the anode. The electrocatalytic method was demonstrated for copper/zinc powder mixtures, gallium arsenide (GaAs) and a sulfidic ore containing gold and silver.
Powder samples of the oxides UO2, UO3, Nd2O3, Eu2O3 and Pr6O11 could be dissolved in the ionic liquid [BMIM][Tf2N] after the addition of HNO3 . This work was carried out to explore the possibility of the direct dissolution of spent nuclear fuel in ionic liquids, with the aim to recover uranium and the rare earths from the ionic liquid by solvent extraction into a supercritical CO2 phase. UO2 could be dissolved oxidatively in different tetrachloroferrate(III) imidazolium ionic liquids, diluted in chloride ionic liquids . Earlier work on the applications of ionic liquids for the processing of spent nuclear fuel have been reviewed by Binnemans . The acidic ionic liquid N,N-dimethylacetamidium bis(trifluoromethylsulfonyl)imide diluted in the ionic liquid [BMIM][Tf2N] was used to dissolve rare-earth oxides, rare-earth carbonates, rare-earth fluorocarbonates, and a bastnasite concentrate prepared by froth flotation . The ionic liquid trihexyl(tetradecyl)phosphonium chloride (Cyphos® IL 101) saturated with concentrated HCl was used to dissolve CaO, NiO, MnO, CoO, CuO, ZnO, and Fe2O3 . The dissolved metals could be selectively stripped by bringing the loaded ionic-liquid phase into contact with aqueous solutions of different chloride concentrations. Ag2O, CuO, ZnO, and NiO could be dissolved in different imidazolium ionic liquids via carbene formation . Perhalide ionic liquids have been used for the oxidative dissolution of metals . Mercury could be dissolved in the ionic liquid 1-butyl-3-methylimidazolium tribromide, [BMIM][Br3]. Also, copper and antimony showed a good solubility in this ionic liquid, whereas aluminum, titanium, and tungsten showed a poor solubility.
Most of the experiments with ionic liquids have been carried out at temperatures below 100 °C. However, some studies showed that ionic liquids with a melting point above 100 °C can also be useful for applications in extractive metallurgy. In 1936, Audrieth and coworkers tested the use of molten pyridinium hydrochloride (formed in a reaction between pyridine and HCl) for the dissolution of metals, metal oxides, and metal salts . Pyridinium hydrochloride has a melting point of 144.5 °C and boils at 219–221 °C. Of the tested metals, Al, Cd, Ca, Mg, Zn, Cu, Mn, Ni, Sn, Pb, and Fe could be dissolved. It is interesting to note that metallic copper can be dissolved in pyridinium hydrochloride, while it cannot be dissolved in concentrated HCl. Of the oxides, Sb2O3, BaO, Bi2O3, CdO, CoO, Cu2O, CuO, Fe2O3, HgO, PbO, MgO, MnO2, NiO, MoO3, and V2O5 were found to be soluble, while WO3 and U3O8 reacted slowly, and Ta2O5, SnO2, ThO2, and TiO2 did not react. The carbonates BeCO3, CaCO3, PbCO3, and MnCO3 reacted readily with pyridinium hydrochloride. Hollebone and coworkers tested molten pyridinium hydrochloride for the treatment of ores, including refractory niobium ores . Finely divided pyrochlore was only poorly soluble (30% dissolved after 18 h at 160 °C), but the Nb2O5 that formed after the fusion of pyrochlore in molten NaOH readily dissolved. After pyridinium hydrochloride was sublimated in vacuum at 180 °C, NbCl5 was obtained. On the other hand, ferrocolumbium readily dissolved in molten pyridinium hydrochloride without any pretreatment. CuS could be dissolved as well, with the release of H2S.
Non-Aqueous Solvent Extraction
Only very few studies on non-aqueous solvent extraction have been reported in the literature, and most have been performed to study fundamental aspects of coordination chemistry in solution and were not aimed at separating mixtures of metal compounds. Earlier authors have recognized the potential of non-aqueous solvent extraction, but the lack of outstanding results led to just a small number of follow-up studies. Nevertheless, non-aqueous solvent extraction offers some interesting opportunities, for instance, the possibility of separating metal compounds that hydrolyze in water.
The distribution of ZrCl4 and HfCl4 between acetonitrile and isoamyl ether was investigated with the aim to separate hafnium from zirconium . However, it was found that the separation factors were too small to be of practical use. Several metal salts (chloride, bromide, thiocyanate, and nitrate) were extracted to a diethyl ether phase that was equilibrated with a second immiscible phase, being ethanolamine, formamide, or adiponitrile . These solvents could extract nearly all metal complexes from the ether phase with an extraction efficiency of more than 90%. Only tin(IV) chloride showed a higher affinity for the ether phase. Thallium(III) was separated from Ga(III), In(III), Fe(III), Sn(II) and Sn(IV) by extracting the elements first from an aqueous 2-M HBr solution with methylisobutyl ketone (MIBK), followed by stripping of the MIBK layer using a 1.5-M HBr solution in formamide . All the thallium(III) remained in the MIBK layer, while all the other metal ions were transferred to the formamide layer. Iron(III) can be extracted from methanol or DMSO using D2EHPA in n-octane . It was observed that equilibrium was reached much more slowly than in the case of extraction from an aqueous solution. Zinc(II) and cadmium(II) were extracted from ethylene glycol (with added HBr or LiBr) using trioctylphosphine oxide (TOPO) dissolved in benzene , while the extraction behavior of zinc(II) was also studied for extraction from ethylene glycol (with added HCl or LiCl) using TOPO dissolved in toluene . A later study investigated the behavior of zinc(II) in the extraction system consisting of diethylene glycol and TOPO dissolved in decaline .
Recently, Foreman studied the extraction of the transition-metal ions and the rare-earth ions from the deep-eutectic solvent choline chloride : lactic acid (1:2) . The transition-metal ions were extracted using the quaternary ammonium salt Aliquat® 336 dissolved in an aromatic diluent and in biodiesel, while the rare-earth ions were extracted using D2EHPA dissolved in aliphatic diluents. The extraction using Aliquat® 336 was found to be more sensitive to the water content of the DES than when using D2EHPA. Batchu et al. developed a solvent-extraction process for rare earths that involved two immiscible organic phases . The more-polar organic phase was ethylene glycol with the dissolved rare-earth nitrate salts and LiNO3, while the less-polar phase was a solution of the neutral extractant Cyanex® 923 dissolved in n-dodecane. Compared with aqueous feed solutions, the light rare-earth elements (LREEs) were less efficiently extracted, and the heavy rare-earth elements (HREEs) were more efficiently extracted from an ethylene glycol feed solution, resulting in a better separation of the HREEs from the LREEs. The separation factors between neighboring elements were higher for extraction from the ethylene glycol solution than those for extraction from an aqueous solution.
Oxidative Dissolution of Metals in Non-Aqueous Solvents
The oxidative dissolution of metals in organic solvents was originally developed for the analysis of alloys, because this method allows for the selective dissolution of the metal, while having little effect on the oxide and other nonmetallic impurities. For instance, bromine-ethyl acetate and bromine-methanol mixtures have been used for the dissolution of uranium alloys. Bromine-methanol has also been used for the dissolution of zirconium, thorium, titanium, and beryllium alloys, and also as an etchant for semiconductors. Many studies have been devoted to the dissolution of gold in organic solvents. Typical solvents are dihalogen-halide-polar aprotic organic solvent (DMF, DMSO, acetonitrile) mixtures [150, 151, 152] or dihalogen-halide-nonpolar solvent (aromatics, chloroform) mixtures [153, 154]. The halide can be an alkali-metal halide or an organic halide salt (e.g., a quaternary ammonium halide). Palladium reacts with iodine in DMF . Mixtures of SOCl2 with pyridine, DMF, pyrimidine, or imidazole are able to dissolve gold, silver, and palladium. These solvents are called “organic aqua regia” because they have similar solvent properties to aqua regia [156, 157]. Interestingly, “organic aqua regia” cannot dissolve platinum, whereas aqua regia can, so that platinum–palladium separations are possible with these organic solvent mixtures. Charge-transfer complexes of dithioxamides with dihalogens are powerful reagents for the dissolution of noble metals [158, 159, 160]. A mixture of iodine and the S-donor tetraethylthiuram disulfide can dissolve gold . DMF-Cl2 can dissolve zirconium , while uranium metal can be dissolved in TBP-TCE-Cl2 or TBP-TCE-NO2 (TBP = tributyl phosphate, TCE = tetrachloroethylene) [163, 164]. As mentioned in the section on ionometallurgical processes, polyhalide ionic liquids with the tribromide anion are able to dissolve elemental mercury .
Solvometallurgy as Part of the Metallurgical Toolbox
Solvometallurgy is a promising new approach to extractive metallurgy with several advantages, but there are still several problems that need to be solved before solvometallurgical processes can be applied on a large scale in industry.
One problem is the high price of the organic solvents and extractants compared with water and mineral acids. Therefore, it is important that these solvents and extractants can be recycled at the end of the process so that the consumption of reagents is a minimum. The recycling of solvents is also mandatory from an environmental point of view. As mentioned elsewhere, it is better not to use distillation for the recovery of solvents, but to use instead more energy-efficient membrane processes.
For health, safety, and environmental reasons, organic solvents that are highly toxic should not be considered for developing solvometallurgical processes. Examples include benzene, nitrobenzene, chloroform, carbon tetrachloride, carbon disulfide, and HMPA. Also solvents with a very low flash point such as diethyl ether must be avoided. Although volatile solvents might seem to be of interest because they can be easily recovered after the reaction by distillation, they should be avoided in open systems. One must be cautious when combining concentrated HNO3 with organic solvents, because concentrated HNO3 is a strong oxidizing agent, and bringing it into contact with organic solvents might cause fires or even explosions. Also protic nitrate ionic liquids can be dangerous when heated .
Ionic liquids and deep-eutectic solvents are very promising classes of solvents for solvometallurgical processes because of their reactivity in solvent leaching, intrinsic electrical conductivity in electrodeposition processes and very low vapor pressure (and hence low flammability and very high flash point). However, these solvents suffer from a high viscosity, especially if their water content is low. A high viscosity hampers the mass transport and slows down the chemical reactions occurring during leaching, solvent extraction, or electrodeposition. A high viscosity also makes solid–liquid separations more difficult. Of course, many aspects of working with viscous liquids are challenging from the chemical engineering point of view.
Solvometallurgy can benefit from knowledge in the fields of coordination chemistry in non-aqueous solvents  or the solvation of ions in non-aqueous solvents . Through a better understanding of the interactions between metal ions or metal complexes and the molecule in the solvent phase, more efficient and selective solvometallurgical processes can be developed. Although an enormous amount of information is available on metal ions in aqueous solutions, very little information is available on metal ions in non-aqueous solvents. Moreover, we must be aware of the fact that even small amounts of water can significantly change the system, especially in those cases where the metal ions have a very strong tendency to bind water molecules, such as in the case of the trivalent rare-earth ions. In anhydrous acetonitrile, acetonitrile molecules will bind to rare-earth ions, but even in the presence of a small amount of water, the rare-earth ions will be coordinated by the water molecules. This is the phenomenon of preferential solvation. This can also occur with other solvent mixtures. For solvometallurgy, a good knowledge of the solvation of metal ions in different solvents and the preferential solvation of these metal ions in solvent mixtures is of great importance.
Comparatively few solvometallurgical processes have been described in the literature, in contrast to the large number of hydrometallurgical and pyrometallurgical processes. Therefore, the full potential of solvometallurgy still needs to be unlocked. So far, no solvometallurgical processes applied in industry have been disclosed (with the exception of the electroplating of aluminum from non-aqueous electrolytes). The Technology Readiness Level (TRL) of solvometallurgical processes is still low. On the TRL scale defined by the European Commission, which ranges from TRL 1 (basic principles observed) to TRL 9 (actual system proven in operational environment), most solvometallurgical processes have a TRL of 3 (experimental proof-of-concept) or 4 (technology validated in the lab). It is important that the sustainability of metallurgical flow sheets with solvometallurgical unit processes is assessed from the very beginning of the process design.
Solvometallurgy is a new branch of extractive metallurgy that can complement pyrometallurgy and hydrometallurgy. Solvometallurgical processes are similar to hydrometallurgical processes, but with the aqueous phase replaced by a non-aqueous phase. Therefore, it is important to realize that conventional solvent extraction cannot be considered as a solvometallurgical process because of the presence of a discrete aqueous phase. An obvious advantage of solvometallurgy is the reduced use of water and the avoidance of problems with wastewater treatment. However, because the solvation of metal ions in organic solvents differs from their solvation (hydration) in water, the efficiency and selectivity of non-aqueous solvent extraction and non-aqueous ion exchange can be different from those observed for the analogous processes with aqueous solvents. By direct solid leaching or non-aqueous-slurry solvent leaching, the processes of leaching and solvent extraction can be combined into a single step, leading to process intensification. However, solvometallurgical processes require a careful selection of the most suitable solvents, and special attention has to be paid to the recovery of solvents after solvent leaching. The solvents must have a low toxicity, a low flammability and a low environmental impact. They should also be biodegradable so that any solvent traces left on the solid residues can be destroyed by heterotrophic microorganisms. This offers the opportunity to combine solvent leaching and bioleaching with heterotrophic microorganisms because these microorganisms can use the solvent traces as nutrients for their growth. The residues obtained after solvent leaching, with or without applying an additional bioleaching step, can be used as the input materials for the preparation of building materials or for cementitious binders. Solvometallurgical unit operations can be considered as part of the metallurgical toolbox for the treatment of low-grade or complex ores, tailings, industrial residues, and urban waste. As such, solvometallurgy can contribute to the integrated, near-zero-waste, metallurgical processing of different secondary resources. The technology readiness level (TRL) of this emerging branch of extractive metallurgy is still low (TRL = 3–4), which is a disadvantage for short-term implementation, but a great opportunity for research, development, and innovation.
The research leading to these results received funding from the European Research Council (ERC) under the European Union’s Horizon2020 Research and Innovation Programme: Grant Agreement 694078—Solvometallurgy for critical metals (SOLCRIMET).
- 1.Habashi F (1997) Handbook of extractive metallurgy. Wiley, WeinheimGoogle Scholar
- 2.Anderson C, Dunne R, Uhrie J (2014) Mineral processing and extractive metallurgy: 100 years of innovation. Society for Mining Metallurgy and Exploration (SME), EnglewoodGoogle Scholar
- 3.Hayes P (2003) Process principles in minerals and materials production, 3rd edn. Hayes Publishing Co, SherwoodGoogle Scholar
- 4.Kimball R, Ewing R (1957) Uranium recovery from ores with hydrochloric acid and acetone. US Patent 2800387Google Scholar
- 5.Grinstead RR (1959) Process for the recovery of metals from high-lime carnotite ores. US Patent 2869980Google Scholar
- 6.Grinstead RR (1958) Process for utilizing organic orthophosphate extractants. US Patent 2860031Google Scholar
- 7.Galvanek P (1959) Process of recovering uranium from its ores. US Patent 2875023Google Scholar
- 8.Bloecher FW Jr (1950) Lyometallurgical tests on Marysvale uranium ores. Mineral Engineering Laboratory, Massachusetts Institute of Technology, Watertown, Report MITG-252Google Scholar
- 9.Bailes R, Magner J (1957) Direct solvent leaching of uranium ores. Mines Mag 47(June):51–54Google Scholar
- 10.Raghavan S, Fuerstenau DW (1993) A lyometallurgical process for leaching copper from chrysocolla. In: Hydrometallurgy fundamentals, technology and innovations, Proceedings of the Milton E., Wordsworth (IV) Int. Symposium on Hydrometallurgy, pp 283–297Google Scholar
- 11.Raghavan S, Harris I, Fuerstenau DW (1979) Lyometallurgical treatment of porous oxidized ores. In: Prepr Pap—Int Miner. Process Congr 13th. Panst. Wydawn. Nauk.-Wroclaw, pp 743–774Google Scholar
- 12.Raghavan S, Harris I, Fuerstenau DW (1981) Lyometallurgical treatment of porous oxidized ores. In: Dev. Miner. Process. pp 960–992Google Scholar
- 13.Tomijima H, Tsukui K, Okoshi Y (1966) Direct dissolution of water-insoluble uranium compounds by contact with neutral organic solvents pretreated with nitric acid. US Patent 3288568Google Scholar
- 14.Sastri V (1975) Selective leaching of metals from ores with organic solvents and chelating agents. J Sci Ind Res 34:663–665Google Scholar
- 15.Marcus Y (1985) Ion solvation. Wiley, New YorkGoogle Scholar
- 16.Chekmarev AM, Chizhevskaya SV, Buchikhin EP (2000) Solvometallurgy as a novel trend in XXI century metallurgy. Khim Tekhnol. 2–7Google Scholar
- 17.Chizhevskaya SV, Chekmarev AM, Klimenko OM, et al (1994) Non-traditional methods of treating high-silicon ores containing rare elements. In: Hydrometallurgy’94. Springer, Dordrecht, pp 219–228. doi: 10.1007/978-94-011-1214-7_13
- 18.Chizhevskaya SV, Chekmarev AM, Povetkina MV, et al (2001) New extraction technologies for the treatment of rare metal raw materials using mechanochemical methods. In: Solvent Extraction for the 21st Century, Proceedings of ISEC ‘99, Barcelona, July 1999, Society of Chemical Industry, London, pp 805–809Google Scholar
- 19.Chekmarev A, Chizhevskaya S, Buchikhin E, Cox M (2001) Solvometallurgical methods in the treatment of rare and non-ferrous metal raw materials. In: Proceedings VI Southern Hemisphere Meeting on Mineral Technology/XVIII Encontro Nacional de Tratamento de Minérios e Metalurgia Extrativa (VI SHMMT/XVIII ENTMM), May 2001, Rio de Janeiro, Brazil, pp 441–444Google Scholar
- 42.Reichardt C (2003) Solvents and solvent effects in organic chemistry, 3rd edn. Wiley, WeinheimGoogle Scholar
- 43.Hecker E (1954) Auswahl von Lösungsmittelsystemen zur Multiplikativen Verteilung. Chimia 8:229–236Google Scholar
- 44.Hecker E (1955) Verteilungsverfahren im Laboratorium. Verlag Chemie, WeinheimGoogle Scholar
- 47.Marcus Y (1973) Ion exchange in nonaqueous and mixed solvents. In: Ion exchange and solvent extraction. Marcel Dekker, New York, pp 1–119Google Scholar
- 48.Katzin L, Sullivan J (1958) Separation of inorganic salts from organic solutions. US Patent 2840451Google Scholar
- 49.Sansoni B (1956) Spezifischer Ionenaustausch durch underschiedliche Solvatation in nichtwässerigen Lösungsmitteln: Kobalt-Nickel-Trennung in geschmolzenem Harnstoff. Angew Chem 68:117–119Google Scholar
- 54.Endres F (2002) Ionic liquids: solvents for the electrodeposition of metals and semiconductors. ChemPhysChem 3:144–154. doi: 10.1002/1439-7641(20020215)3:2<144:AID-CPHC144>3.3.CO;2-R CrossRefGoogle Scholar
- 73.Hughes C, Whale G, Mead C (2015) Investigation into the biodegradability of various hydrocarbon solvents. Royal Dutch Shell Report 1–1Google Scholar
- 93.Brown P, Jacob S (1981) Process for purification of lithium chloride. US Patent 4274834Google Scholar
- 94.Ewing R, Kiehl S, Bearse A (1955) Nonaqueous extractive methods for Western uranium ores. Final report to the U.S. Atomic Energy Commission, Contract No. AT-(49-1)-635, Battelle Memorial Institute, Columbus OhioGoogle Scholar
- 95.Rosenbaum J, Clemmer J, Lennemann W (1956) Innovation in processing uranium ores. Final report to the U.S. Atomic Energy Commission, Contract No. AT-(49-1)-635, Bureau of Mines. Intermountain Experiment Station, Salt Lake CityGoogle Scholar
- 96.Parker A (1973) Hydrometallurgy of copper and silver in solvent mixtures. Search 4:426–432Google Scholar
- 97.Parker A (1972) Solvation of ions—some applications. Proc R Aust Chem Inst 39:163–170Google Scholar
- 100.Preston J, Muir D, Parker A (1980) Cuprous hydrometallurgy 8. Solvent extraction and recovery of copper(I) chloride with organic nitriles from an iron(III), copper(II) chloride, 2-step oxidative leach of chalcopyrite concentrate. Hydrometallurgy 5:227–241. doi: 10.1016/0304-386X(80)90041-9 CrossRefGoogle Scholar
- 108.Thorsen G (1980) Extraction and separation of metals from solids using liquid cation exchangers. US Patent 4200504Google Scholar
- 117.Davris P, Balomenos E, Panias D, Paspaliaris I (2014) Leaching of rare earths from bauxite residues using imidazolium ionic liquids. In: Proceedings of the 1st European Rare Earth Resources Conference (ERES 2014), Milos (Greece), 4–7 September 2014, pp 241–252Google Scholar
- 118.Davris P, Balomenos E, Panias D, Paspaliaris I (2015) The use of ionic liquids for rare earth element extraction from bauxite residue. In: Proceedings of the Bauxite Residue Valorisation and Best Practices Conference 2015, Leuven (Belgium), 5–7 October 2015, pp 323–330Google Scholar
- 123.Kiliçarslan A, Saridede MN (2015) Application of 1-methylimidazolium hydrogen sulfate ionic liquid to the oxidative leaching of copper and zinc in industrial brass dross. In: Energy technology 2015. The Minerals, Metals & Materials Society, Warrendale; John Wiley & Sons, Hoboken, pp 209–215. doi: 10.1002/9781119093220.ch23
- 139.Rogers R, Holbrey J (2012) Ionic liquid solvents of perhalide type for metals and metal compounds. US Patent Application 20120090430Google Scholar
- 141.Hollebone B, Morgan W, Wiles D (1967) The use of molten pyridinium chloride in the thermal treatment of ores of niobium (columbium) and other refractory metals. Trans Metall Soc AIME 239:97–99Google Scholar
- 145.Borshch N (1987) Extraction of iron(III) from polar nonaqueous solvents and some particularities of liquid extraction of metal ions in such systems. J Anal Chem USSR 42:857–861Google Scholar
- 146.Matsui M, Aoki T, Inoue O, Shigematsu T (1975) Nonaqueous liquid-liquid extraction. Extraction of zinc and cadmium from ethylene glycol solution of bromide by trioctylphosphine oxide. Bull Inst Chem Res Kyoto Univ 52:652–657Google Scholar
- 153.Nakao Y (1991) Dissolution of metals in halogen cetylpyridinium halide-benzene systems. J Chem Res S 228–229Google Scholar
- 155.Buchikhin E, Kuznetsov A, Chekmarev A, Lavrent’ev I (1999) Reaction of metallic palladium with iodine in dimethylformamide. Russ J Coord Chem 25:416–417Google Scholar
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.